Research Article  Open Access
Yijun Wang, Liuding Wang, Cheng Yan, "Field Emission Properties of Carbon Nanotubes with Boron Doping and H_{2}O Adsorption", Journal of Nanomaterials, vol. 2013, Article ID 404923, 6 pages, 2013. https://doi.org/10.1155/2013/404923
Field Emission Properties of Carbon Nanotubes with Boron Doping and H_{2}O Adsorption
Abstract
Gas adsorption and atom doping usually present when preparing carbon nanotubes (CNTs) and can affect the field emission properties of carbon nanotubes. H_{2}O molecule and boron atom are the most important adsorbates, respectively. Using abinitio calculations, we have investigated the electron field emission performance of CNTs simultaneously adsorbed with one H_{2}O molecule and doped with one boron atom (BCNT+H_{2}O) in this paper. The results indicate that the electrons localize at the top of BCNT+H_{2}O and the electronic density of states (DOS) around the Fermi level is enhanced obviously. It is expected that BCNT+H_{2}O will be more propitious to the field emission of electrons based on the calculations of DOS, HOMO/LUMO, and Mulliken charge population.
1. Introduction
Carbon nanotubes (CNTs) have attracted much attention due to their high aspect ratio and remarkable mechanical, electronic, and chemical properties [1–3]. The quasionedimensional structures and unique electric properties make CNTs have a lot of potential applications in different fields [4–6]. Especially, because of the excellent field emission properties, CNTs have been promising candidates for flatpanel displays [7, 8]. Up to now, many experimental [9] and theoretical [10–12] studies have shown that the gas adsorption is of great advantage to the electron emission of the CNTs. For example, Kim et al. calculated the DOS and field emission properties of closed CNTs under electric field [13], Maiti et al. explained the reason why H_{2}O adsorption on the top of CNTs can improve the electron emission properties [14], and Zhang et al. pointed out that CNTs doped with boron and nitrogen are easy to emit electrons [15].
Naturally, some kinds of gas can markedly change the energy band structure of carbon nanotubes, whereas the work of simultaneous doping and adsorption is rarely reported until now. Therefore, it is very important to study the emission properties of CNTs doped with other atoms and adsorbed with gases under electric field. In this paper we adopted the density functional theory (DFT) to investigate the performances of BCNT+H_{2}O.
2. Models and Calculation Methods
A singlewalled armchair (5, 5) CNT with a cap (Figure 1) is adopted. The cap is a hemisphere (30 carbon atoms) of C_{60} at one end of the CNT and the dangling bonds at the other end are saturated by hydrogen atoms. The position of boron dope is selected at the top layer of the CNT and the distance of H_{2}O adsorption from the top pentagon is about 0.3 nm. Therefore the whole system contains 93 atoms.
(a)
(b)
(c)
(d)
All the calculations were carried out by using firstprinciple DFT provided by DMOL^{3} code [16]. The geometrical optimization was based on the local density approximation (LDA) during selfconsistent field iteration with the PerdewWang parameterization of the local exchange correlation energy. The generalized gradient approximation (GGA) was adopted to calculate the total energy and various electronic properties with the PerdewWang91 (PW91) function [17]. The allelectron KohnSham wave functions were expanded in the local atomic orbital basis set with orbital cutoff of 4.5 Å. Selfconsistent field procedure was done with a convergence criterion of 10^{−5} a.u. on the energy and electron density.
3. Results and Discussion
In order to study the electronic field emission properties of BCNT+H_{2}O, a uniform external electric field with the direction from the top to the end of the CNT is applied, whose intensities are and eV/nm, respectively. In real field emission conditions, a short tip of the structures is considered. The electric field gradient along CNTs axis is ignored and the whole structure is supposed to be in a uniform external electric field [17].
The adsorption distance and adsorption energy are shown in Table 1. The adsorption energy () under the different electric field is defined in (1) and (2), respectively. Consider the following: where the , , and are the total energy of the pure CNT, the adsorbate (a H_{2}O molecule), and the adsorbed CNT system, respectively, under the strength of electric field of 0 eV/nm, and where and have the same meaning under the strength of electric field of 10 eV/nm.

From Table 1, we can see that the adsorption distance is about 0.3 nm and the adsorption energy is very small for BCNT+H_{2}O and CNT+H_{2}O systems in the absence of electric field. When the electric field increases to 10 eV/nm, their adsorption energy is remarkably enhanced, while their adsorption distance decreases slightly. Moreover, Table 1 shows that the adsorption energy of BCNT+H_{2}O is much higher than that of CNT+H_{2}O under the same strength of electric field, which indicates that the structure of BCNT+H_{2}O is more stable [18] than that in a electron transmitter.
Figure 2 presents the DOS of the two systems under the different electric fields and the local density of states (LDOS) of the boron atom and the nearest three carbon atoms on the top of BCNT+H_{2}O under eV/nm. Obviously, the DOS plots of the two systems shift towards the low energy direction and their corresponding peak positions of antibond states are more close to when the electric fields increase from 0 to 10 eV/nm. This indicates that the probability of electron occurrence at antibond states increase, which is well consistent with Kim’s conclusion [13].
(a)
(b)
(c)
(d)
(e)
To determine the pseudogap, an advanced peak separation technique [19] is adopted. Furthermore, the DOS at is also calculated, as listed in Table 2. When the electric fields increase from 0 to 10 eV/nm, the DOS of the two systems at enhances by a big margin. Especially the DOS of BCNT+H_{2}O is about 179% that of CNT+H_{2}O at eV/nm. The reasons can be found from Figure 2(e) that the peak position of LDOS for BCNT+H_{2}O tip is very close to Fermi level, which leads to the enhancement of DOS at . Moreover, we can infer that the external electric field significantly weakens the covalent bond and enhances the metallic bond from the pseudogap of BCNT+H_{2}O compared with CNT+H_{2}O. Therefore, the calculated results and theoretical analysis above mentioned indicate consistently that the electron transmission in BCNT+H_{2}O is much easier and the corresponding field emission properties can be effectively improved compared with CNT+H_{2}O.

To further investigate the field emission property of BCNT+H_{2}O, we have performed the electronic orbital analysis. As shown in Figure 3, the HOMOs of CNT+H_{2}O and BCNT+H_{2}O are all localized at their body and the distribution is very similar no matter whether the electric field is applied or not. However, the LUMO of later is mainly localized at the tip of CNTs at eV/nm.
(a)
(b)
(c)
(d)
(e)
(f)
(g)
(h)
This means that there are more electrons congregating on the top region of BCNT+H_{2}O. Once the stronger electric field is applied these electrons immediately emit to the surrounding space. It can be seen that the conclusions of orbital analysis are well consistent with that of the discussion above.
When a boron atom substitutes a carbon atom in the top layer, the charges distribution and the electronic structures change accordingly. Figure 4 exhibits the results of Mulliken population analysis for the CNT+H_{2}O and BCNT+H_{2}O in the presence of eV/nm. We can see that the boron atom carries a little negative charge and each of the nearest three carbon atoms carries much more negative charges than other atoms located in the first and second layer [20]. The analysis results show that the boron doping can cause more electrons aggregation at the top. Essentially, the electron congregation becomes more obvious with the increase of applied electric field and extra electrons on the tip of system will congregate in the conduction band. Consequently the Fermi level shifts toward the vacuum level. This will lower the potential barrier of BCNT+H_{2}O tip and make the field emission more easily. All of these discussions indicate that BCNT+H_{2}O can enhance the electron field emission.
(a)
(b)
4. Conclusions
In summary, we investigate the electronic structure and physical mechanism of the fieldemission of the capped SWNT which are simultaneously adsorbed with one H_{2}O molecule and doped by a boron atom in the top layer. The calculations and analysis confirm that BCNT+H_{2}O has a higher DOS at than CNT+H_{2}O. Although the HOMO of BCNT+H_{2}O changes hardly with and without the applied electric field, the LUMO is highly localized at the top. Furthermore, the Mulliken population analysis shows that a lot of electrons congregate at the cap of BCNT+H_{2}O. Naturally, present results of the LDOS, the pseudogap, the HOMO/LUMO, and Mulliken population analysis congruously indicate that BCNT+H_{2}O can effectively improve the fieldemission properties of carbon nanotubes compared with CNT+H_{2}O.
Conflict of Interests
The authors, hereby, declare that they do not have any conflict of interests.
Acknowledgments
This work was financially supported by the National Natural Science Foundation of China (11075135, 61307002), the Natural Science Foundation of Shaanxi Province (no. 2012JM1009), the Scientific Research Program of Shaanxi Provincial Education Department (no. 12JK0984), the Scientific Research Program (nos. 12XSYK014, 12XSYK017), and the Teaching Reform Research Program of Xianyang Normal University (no. 201200127), China.
References
 S. Iijima, “Helical microtubules of graphitic carbon,” Nature, vol. 354, no. 6348, pp. 56–58, 1991. View at: Google Scholar
 C. Hierold, O. Brand, G. K. Fedder, J. G. Korvink, and O. Tabata, Carbon Nanotube Devices: Properties, Modeling, Integration and Applications, vol. 8 of Advanced Micro & Nanosystems, WileyVCH, 2008.
 A. V. Eletskii, “Carbon nanotubebased electron field emitters,” PhysicsUspekhi, vol. 53, no. 9, pp. 863–892, 2010. View at: Publisher Site  Google Scholar
 J. Ali, A. Kumar, S. Husain, M. Kumari, H. Harsh, and M. Husain, “Characterization and field emission studies of uniformly distributed multiwalled carbon nanotubes (MWCNTS) film grown by lowpressure chemical vapour deposition (LPCVD),” Current Nanoscience, vol. 7, no. 3, pp. 333–336, 2011. View at: Publisher Site  Google Scholar
 S. M. Lupekhin and A. A. Ibragimov, “Field emission of electrons from a single carbon fiber with a nanostructured emitting surface,” Technical Physics, vol. 57, no. 1, pp. 119–123, 2012. View at: Publisher Site  Google Scholar
 E. F. Zharikova, L. I. Ochertyanova, I. V. Vasylenko et al., “Multiwalled carbon nanotubes with the pyridinecontaining fragment and copper(II) ions,” Russian Chemical Bulletin, vol. 61, no. 7, pp. 1430–1436, 2012. View at: Google Scholar
 V. Guglielmotti, E. Tamburri, S. Orlanducci et al., “Macroscopic selfstanding SWCNT fibres as efficient electron emitters with very high emission current for robust cold cathodes,” Carbon, vol. 52, no. 2, pp. 356–362, 2013. View at: Google Scholar
 N. PereaLópez, B. RebolloPlata, J. A. BrionesLeón et al., “Millimeterlong carbon nanotubes: outstanding electronemitting sources,” ACS Nano, vol. 5, no. 6, pp. 5072–5077, 2011. View at: Publisher Site  Google Scholar
 X. P. Tang, A. Kleinhammes, H. Shimoda et al., “Electronic structures of singlewalled carbon nanotubes determined by NMR,” Science, vol. 288, no. 5465, pp. 492–494, 2000. View at: Publisher Site  Google Scholar
 S. Seenithurai, R. K. Pandyan, S. V. Kumar, and M. Mahendran, “H_{2} adsorptionin Ni and passivated Ni doped 4 Å single walledcarbon nanotube,” International Journal of Hydrogen Energy, vol. 38, no. 18, pp. 7376–7381, 2013. View at: Google Scholar
 M. O. Ezzat, O. H. S. AlObaidi, and M. N. Mordi, “Theoretical study of benzylic oxidation and effect of para—substituents by using hyperchem program,” Journal of Proteomics and Bioinformatics, vol. 4, no. 5, pp. 113–115, 2011. View at: Publisher Site  Google Scholar
 B. Lu and Z. Zhen, “Computational study of B or Ndoped singlewalled carbon nanotubes as NH_{3} and NO_{2} sensors,” Carbon, vol. 45, no. 10, pp. 2105–2110, 2007. View at: Publisher Site  Google Scholar
 C. Kim, B. Kim, S. M. Lee, C. Jo, and Y. H. Lee, “Electronic structures of capped carbon nanotubes under electric fields,” Physical Review B, vol. 65, no. 16, pp. 165418–165423, 2002. View at: Google Scholar
 A. Maiti, J. Andzelm, N. Tanpipat, and P. Von Allmen, “Effect of adsorbates on field emission from carbon nanotubes,” Physical Review Letters, vol. 87, no. 15, Article ID 155502, 2001. View at: Google Scholar
 G. Zhang, W. Duan, and B. Gu, “Effect of substitutional atoms in the tip on fieldemission properties of capped carbon nanotubes,” Applied Physics Letters, vol. 80, no. 14, pp. 2589–2591, 2002. View at: Publisher Site  Google Scholar
 B. J. Delley, “DMOL is available commercially from BIOSYM technologies,” Chemical Physics, vol. 92, pp. 508–517, 1990. View at: Google Scholar
 L. Qiao, W. T. Zheng, H. Xu, L. Zhang, and Q. Jiang, “Field emission properties of Ndoped capped singlewalled carbon nanotubes: a firstprinciples densityfunctional study,” Journal of Chemical Physics, vol. 126, no. 16, Article ID 164702, 2007. View at: Publisher Site  Google Scholar
 Z. Li and C. Y. Wang, “Firstprinciples study of field emission properties of gas adsorption on the carbon nanotubes,” Chemical Physics, vol. 330, no. 3, pp. 417–422, 2006. View at: Publisher Site  Google Scholar
 L. D. Wang, J. Q. Zhou, Q. X. Cao, and Z. Chen, “Investigation of peak separation for Xray diffraction profiles of spinodal decomposition by a kind of optimized Voigt function,” Journal of Materials Science and Technology, vol. 19, no. 4, pp. 371–373, 2003. View at: Google Scholar
 Y. J. Wang, L. D. Wang, M. Yang, and C. Yan, “Effects of B and N dopings and H_{2}O adsorption on structural stability and field emission properties of conecapped carbon nanotubes,” Chinese Physics B, vol. 20, no. 11, Article ID 117304, 2011. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2013 Yijun Wang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.